- Electron beam physical vapor deposition
Electron Beam Physical Vapor Deposition or EBPVD is a form of
physical vapor depositionin which a target anode is bombarded with an electron beam given off by a charged tungsten filament under high vacuum. The electron beam causes atoms from the target to transform into the gaseous phase. These atoms then precipitate into solid form, coating everything in the vacuum chamber with a thin layer of the anode material.
Thin film depositionisired properties.The deposition process can be broadly classified into physical vapor deposition(PVD) and chemical vapor deposition(CVD). In CVD, the film growth takes place at high temperatures, leading to the formation of corrosive gaseous products, and it may leave impurities in the film. The PVD process can be carried out at lower deposition temperatures and without corrosive products, but deposition rates are lower and it leaves residual compressive stress in the film. Electronbeam physical vapor deposition, however, yields a high deposition rate from 0.1 μm/ min to 100 μm / min at relatively low substrate temperatures, with very high material utilization efficiency. The schematic of an EBPVD system is shown in Fig 1.
Thin film deposition process
In an EBPVD system, the deposition chamber is evacuated to a
pressureof 10-4 Torr. The material to be evaporated is in the form of ingots. There are as many as six electron guns, each having a power from few tens to hundreds of kW. Electron beams can be generated by thermionic emission, field emissionor the anodic arc method. The generated electron beam is accelerated to a high kinetic energy and focused towards the ingot. When the accelerating voltage is between 20 kV – 25 kV and the beam current is a few amperes, 85% of the kinetic energy of the electrons is converted into thermal energy as the beam bombards the surface of the ingot. The surface temperature of the ingot increases resulting in the formation of a liquid melt. Although some of incident electron energy is lost in the excitation of X-rays and secondary emission, the liquid ingot material evaporates under vacuum.
The ingot itself is enclosed in a
coppercrucible, which is cooled by watercirculation. The level of molten liquid pool on the surface of the ingot is kept constant by vertical displacement of the ingot. The number of ingot feeders depends upon the material to be deposited. The evaporation rate may be of the order of 10-2 g/cm2 sec.
Material evaporation methods
Refractorycarbides like titanium carbideand borides like titanium borideand zirconium boride can evaporate without undergoing decomposition in the vapor phase. These compounds are deposited by direct evaporation. In this process these compounds, compacted in the form of an ingot, are evaporated in vacuum by the focused high energy electron beam and the vapors are directly condensed over the substrate. Certain refractory oxides and carbides undergo fragmentation during their evaporation by the electronbeam, resulting in a stoichiometry that is different from the initial material. For example, alumina, when evaporated by electron beam, dissociates into aluminum, AlO3 and Al2O. Some refractory carbides like silicon carbide and tungsten carbide decompose upon heating and the dissociated elements have different volatilities. These compounds can be deposited on the substrate either by reactive evaporation or by co-evaporation. In the reactive evaporation process, the metalis evaporated from the ingot by the electron beam. The vapors are carried by the reactive gas, which is oxygen in case of metal oxides or acetylenein case of metal carbides. When the thermodynamic conditions are met, the vapors react with the gas in the vicinity of the substrate to form films. Metal carbide films can also be deposited by co- evaporation. In this process, two ingots are used, one for metal and the other for carbon. Each ingot is heated with a different beam energy so that their evaporation rate can be controlled. As the vapors arrive at the surface, they chemically combine under proper thermodynamic conditions to form a metal carbide film.
The substrate on which the film deposition takes place is ultrasonically cleaned and fastened to the substrate holder. The substrate holder is attached to the manipulator shaft. The manipulator shaft moves translationally to adjust the distance between the ingot source and the substrate. The shaft also rotates the substrate at a particular speed so that the film is uniformly deposited on the substrate. A negative bias D.C.
voltageof 200 V – 400 V is applied to the substrate Focused high energy electrons from one of the electron guns preheat the substrate.
Ion beam assisted deposition
EBPVD systems are equipped with ion sources. These
ionsources are used for substrate etching and cleaning, sputteringthe target and controlling the microstructureof the substrate. The ion beams bombard the surface and alter the microstructure of the film. When the deposition reaction takes place on the hot substrate surface, the films develop an internal tensile stress due to the mismatch in the coefficient of thermal expansion between the substrate and the film. High energy ions can be used to bombard these ceramic thermal barrier coatings and change the tensile stressinto compressive stress. Ion bombardment also increases the density of the film, changes the grain size and modifies amorphous films to polycrystallinefilms. Low energyions are used for the surfaces of semiconductor films.
Advantages of EBPVD
The deposition rate in this process can be as low as 1 nm per minute to as high as few micrometers per minute. The material utilization efficiency is high relative to other methods and the process offers structural and morphological control of films. Due to the very high deposition rate, this process has potential industrial application for
wearresistant and thermal barrier coatings in aerospace industries, hard coatings for cuttingand toolindustries, and electronic and opticalfilms for semiconductor industries.
Disadvantages of EBPVD
EBPVD is a line-of-sight of deposition process. The translational and rotational motion of the shaft helps for coating the outer surface of complex geometries, but this process cannot be used to coat the inner surface of complex geometries. Another potential problem is that filament degradation in the electron gun results in a non-uniform evaporation rate.
# D. Wolfe, Thesis (Ph.D), Thesis 2001dWolfe,DE, Synthesis and characterization of TiC, TiBCN,TiB2 /TiC and TiC/CrC multilayer coatings by reactive and ion beam assisted, electron beam-physical vapor deposition (EB-PVD) The Pennsylvania State University, 1996.
Wikimedia Foundation. 2010.
Look at other dictionaries:
Electron beam physical vapor deposition — Traduction à relire Electron beam physical vapor deposition → … Wikipédia en Français
Physical vapor deposition — (PVD) is a variety of vacuum deposition and is a general term used to describe any of a variety of methods to deposit thin films by the condensation of a vaporized form of the material onto various surfaces (e.g., onto semiconductor wafers). The… … Wikipedia
Physical vapor deposition — Der Begriff physikalische Gasphasenabscheidung (englisch physical vapour deposition, kurz PVD) bezeichnet eine Gruppe von vakuumbasierten Beschichtungsverfahren bzw. Dünnschichttechnologien, bei denen im Gegensatz zu CVD Verfahren die Schicht… … Deutsch Wikipedia
Thin-film deposition — is any technique for depositing a thin film of material onto a substrate or onto previously deposited layers. Thin is a relative term, but most deposition techniques allow layer thickness to be controlled within a few tens of nanometers, and some … Wikipedia
Evaporation (deposition) — Evaporation machine used for metallization at LAAS technological facility in Toulouse, France. Evaporation is a common method of thin film deposition. The source material is evaporated in a vacuum. The vacuum allows vapor particles to travel… … Wikipedia
Environmental scanning electron microscope — Wool fibers imaged in an ESEM by the use of two symmetrical plastic scintillating backscattered electron detectors … Wikipedia
Ion beam — An ion beam is a type of particle beam consisting of ions. Ion beams have many uses in electronics manufacturing (principally ion implantation) and other industries. Today s ion beam sources are typically derived from the mercury vapor thrusters… … Wikipedia
Coating — is a covering that is applied to the surface of an object, usually referred to as the substrate. In many cases coatings are applied to improve surface properties of the substrate, such as appearance, adhesion, wetability, corrosion resistance,… … Wikipedia
List of coating techniques — This list contains an overview of coating techniques for thin film deposition, found in the field of materials science. The techniques can be classified as follows: Chemical vapor deposition (CVD) * Metalorganic vapour phase epitaxy *… … Wikipedia
Tunnel magnetoresistance — Magnetic tunnel junction (schematic) The Tunnel magnetoresistance (TMR) is a magnetoresistive effect that occurs in magnetic tunnel junctions (MTJs). This is a component consisting of two ferromagnets separated by a thin insulator. If the… … Wikipedia